Binding studies of creatinine and urea on iron-nanoparticle
© Banerji and Pramanik. 2015
Received: 3 September 2015
Accepted: 20 October 2015
Published: 19 November 2015
Kidney diseases are complicated and can be fatal. Dialysis and transplantation are the only survival solutions to the patients suffering from kidney failures. Both hemodialysis and peritoneal dialysis are risky, due to the possibility of infection and these are expensive and time consuming. The development of simple and reliable technique for the clearance of creatinine and urea from the body is an important part of biotechnology. We have synthesized an iron nanoparticle (INP) and studied its binding with creatinine and urea. The DLS, TEM, AFM, FT-IR and Powder-XRD studies demonstrate strong binding of creatinine and urea to the nanoparticles. This finding may be helpful if it is used in the dialysis technologies. The proposed method may substantially decrease dialysis time and improve its quality in terms of urea and creatinine clearances.
Chronic kidney disease (CKD) is becoming increasingly common and can lead to chronic kidney failure when both the kidneys stop functioning totally (Dousdampanis et al. 2014; Rahbari-Oskoui et al. 2014). The kidneys are filtration units which purify blood from the waste by-products including creatinine and urea. Eventually in the case of kidney failure these and other waste molecules accumulate in the body and dialysis becomes the only solution (Kim and Takayama 2015; Nassar and Ayus 2001). To date no proper medicine has emerged for the treatment of CKD, with the exception of strong immuno-suppressant drugs which actually prolong the kidney failure rather than effect a cure (Nassar and Ayus 2001; Dalal et al. 2011). Dialysis is associated with a high risk of infection and is costly (Nassar and Ayus 2001).
Among various nanoparticles, iron nanoparticles (INPs) have been found to be biologically compatible, and can be coated with biomolecules, drugs, enzymes, or antibodies to increase their functionalities for bio-sensing applications (Xie et al. 2010; Todd et al. 2014; Bachelet-Violette et al. 2014; Verma et al. 2014). It is cheap, non-toxic, and easy to prepare (Tromsdorf et al. 2009; Banerji et al. 2012a, b). Now a days INPs have been widely used for targeted drug delivery, immobilization of enzymes, biosensor, and different environmental analysis (Verma et al. 2014). They are extensively used as MRI contrast agents due to their ability to shorten T2* relaxation times for the liver, spleen, and bone marrow (Na et al. 2009). The surface properties of INPs allow to functionalize with small organic molecules by their various functional groups for wide range of applications (Weingart et al. 2013). The nano-bio composite of INPs and chitosan have been reported for the detection of glucose, urea, phenolic compounds and ferritin (Lin et al. 2015). However, immobilization of biomolecules onto surface charged super paramagnetic INPs are of great interest because of magnetic behavior of their bio conjugates (Wahajuddin 2012).
Recently, we have initiated a program to synthesize iron-nanoparticles (INPs) with high affinity towards nitrogen containing compounds (Banerji et al. 2012a). With an aim to test the use of the INPs for the treatment of CKD patients, we have studied the binding affinity of creatinine and urea using various techniques like DLS, TEM, AFM, FT-IR and Powder-XRD. Here we disclose our preliminary results on the binding studies of creatinine and urea on INPs. One future possibility of this study is to utilize the strong affinity binding of creatinine and urea into the dialysis technology. It is proposed that in the presence of nanoparticles the rate of osmosis may be much higher compared to normal case leading to better dialysis. The present study thus may be the first foot-step towards achieving that major goal.
FeCl2·4H2O, FeCl3·6H2O, urea and creatinine were purchased from Sigma Aldrich. Sodium hydroxide (NaOH), hydrochloric acid (HCl), citric acid and sodium citrate were obtained from Merck. Carbon coated copper grid for TEM study was purchased from Allied Scientific Product, USA. ASTM V1 Grade Ruby Mica sheet for AFM study was purchased from Micafab India Pvt. Ltd., Chennai, India. Water obtained from Sartorius Stedim biotech machine was used for all the experiments.
Synthesis of iron-nanoparticles
First 1 g (0.005 mol) FeCl2·4H2O was dissolved in 20 ml 1 (M) HCl and then 2.7 g (0.01 mol) FeCl3.6H2O was added to the solution and stirred under magnetic stirrer. Then 2 (M) NaOH solution was added until the black precipitate appeared and the pH also become basic. This black precipitate was then separated and washed three times with 30 ml deionized and deoxygenated water. After that 20 ml citric acid-sodium citrate buffer was added to disperse the INPs. These INPs were washed by repeated cycles (four times) of centrifugation and dried in air. Millipore water was used throughout to disperse the nanoparticles as needed for characterization as well as further studies.
Synthesis of iron-nanoparticle-creatinine and iron-nanoparticle-urea conjugates (Chen and Kimura 1999; Brust et al. 1994)
Creatinine and urea bind to the INPs by noncovalent interaction (van der Waals forces) between the INPs and creatinine/urea. Creatinine/urea solution of concentration 0.5 mg/ml was prepared by dissolving 50 mg of creatinine/urea in 100 ml millipore water. For the conjugation of creatinine/urea onto iron nanoparticles (INPs), 10 ml of this solution and 20 mg of as-synthesized INPs were taken into a flat-bottomed conical flask with glass stopper. The flask was sealed with parafilm and stirred at 60 °C for 24 h. The unbound creatinine and urea were separated by centrifugation at 30,000 rpm for 30 min. The conjugated INPs were washed by repeated cycles of centrifugation and dried under vacuum.
Dynamic light scattering (DLS)-based zeta-potential measurements (Kuypers et al. 2015)
To obtain an idea about the size distributions and stability of INPs, creatinine conjugated INPs and urea conjugated INPs, DLS experiments (model: Zetasizer Nano Z, Malvern Instruments Ltd, United Kingdom) were carried out with their aqueous suspension at 20 °C. The scattered lights were collected at a 90o angle. Data were acquired and analyzed by Precision Deconvolve program. For a typical DLS experiment, 200 μl (conc. 2 mg/ml) of a sample solution was slowly pipetted into a clean quartz micro-cuvette.
TEM sample preparation and imaging (Banerji et al. 2014)
A Tecnai G2 Spirit TEM operating at 80 kV was used to study the morphology of the INPs and conjugated INPs. 10 µl (conc. 2 mg/ml) of the nanoparticle solution was placed on a 300-mesh carbon coated copper grid (formvar foil upon copper grids) and the excess samples were removed cautiously by tissue paper. No additional staining was done.
AFM sample preparation and imaging (Banerji et al. 2012a)
10 µl (conc. 2 mg/ml) of the nanoparticle solution was deposited on a freshly cleaved muscovite Ruby mica sheet 10 min after that the sample was dried under vacuum. AC-mode atomic force microscopy was performed by using a Pico Plus 5500 AFM (Agilent Technologies, Inc., Santa Clara, CA, USA) with a piezo scanner maximum range of 9 μm. Microfabricated silicon cantilevers of 225 μm in length with a nominal spring force constant of 21–98 N/m were used from nanosensors. Cantilever oscillation frequency was tuned into resonance frequency. The cantilever resonance frequency was 150–300 kHz. All the images (512 × 512 pixels) were captured with a scan size between 0.5 and 5 μm at the scan speed rate of 0.5 rpm. The images were processed by flattening using Pico view software (Molecular Imaging Inc., Ann Arbor, MI, USA).
FT-IR experiment (Banerji et al. 2013)
The FT-IR spectra of the samples were recorded on a JASCO FT/IR 4200 spectrometer using the (KBr) disc technique. For FT-IR measurements all the samples are used in their solid powder form. The solid creatinine, urea, creatinine conjugated INPs and urea conjugated INPs were mixed with KBr separately in a clean glass mortar and compressed to obtain a pellet. Background spectra were obtained with a KBr pellet for each sample. JASCO software was used for data processing.
Powder X-Ray diffraction study
X-Ray diffraction studies of INPs, creatinine tagged INPs and urea tagged INPs were carried out with a Scifert X-ray diffractometer (C 3000) using ‘Cu ka’ radiation. The data collection was recorded in the range of 2θ = 5–60° with a step of 0.02o and 2 s/step.
Results and discussion
The average diameters and the size distribution polydispersity index (PDI) of the samples were determined by DLS. DLS experiments were carried out with their aqueous solutions and the results showed that the mean particle size of INPs (intensity average) are 8.66 ± 4 nm with PDI 0.23, creatinine tagged INPs are 9.26 ± 3 nm with PDI 0.29 and that of urea tagged INPs are 9.16 ± 4 nm with PDI 0.34. The zeta potential distribution of INPs are negative charged to −38.8 mV, creatinine tagged INPs with a negative charge −23.5 mV and of urea tagged INPs with a negative charge −21.4 mV in water, which are sufficient to keep the particles from interacting with each other and therefore maintain a stable particle size of the sample. The decrease in zeta potential of INPs is observed due to the coating of creatinine/urea over INPs which minimizes the free surface energy by restructuring the surface (Nel et al. 2009). The resulting negative charges in INPs, creatinine tagged INPs and urea tagged INPs are attributed to negative surface charge on them.
TEM and AFM imaging
Interpretation of FT-IR spectra
X-ray diffraction study
For all the reflections correspond to INPs are very close to those of the standard data of Fe3O4 alone in powder diffraction PDF card (JCPDS No. 82n1533) (Banerji et al. 2012a). The presence of sharp and intense peaks confirmed the formation of highly crystalline INPs. The appearance of sample diffraction peaks at 2θ = 30.16°, 35.70°, 43.33°, 53.60°, 57.10°, and 62.9° corresponded to the (220), (311), (400), (422), (511) and (440) crystal planes of Fe3O4 respectively, which indicated that the resulting particles were Fe3O4, with structures of cubic crystal (Banerji et al. 2012). The X-ray diffraction pattern and the main diffraction angles of creatinine tagged INPs agreed with the data of creatinine. However, for creatinine tagged INPs the intensities of the diffraction peaks at 2θ = 7.4°, 19.9°, 25.8°, and 27.5° are due to the (100), (200), (300), (012) and (013) planes of creatinine molecule (Sakata et al. 2005). In case of urea tagged INPs the main diffraction angles agreed with the data of urea. However, the intensities of the diffraction peak at 2θ = 22.6°, 33.1° and 65.5° are corresponds to the (110), (210) and (212) planes of urea (Fernández-Bertrán et al. 2000). For creatinine tagged INPs and urea tagged INPs the indices corresponding to Fe3O4 are present. This reveals that the modification of INPs surface with creatinine or urea does not result in the phase change of Fe3O4.
Application and future scopes
The INPs are nontoxic in nature to the human body which was earlier reported by our group (Banerji et al. 2012a). The binding of creatinine and urea into the INPs may be useful for the dialysis patients if this basic research is successfully translated and applied into dialysis technology. Dialysis is based on the principle of osmosis and the rate of osmosis may be enhanced by employing INPs externally into the dialyzer. It is proposed that the INPs may capture more creatinine and urea from the blood thereby shifting the equilibrium more towards right. Hence it is believed that urea and creatinine clearance may improve, this way by making the dialysis more efficient.
All the analytical techniques (DLS, TEM, AFM, FT-IR, and Powder-XRD) have unambiguously proved the strong binding of creatinine and urea with INPs. In our laboratory, currently we are pursuing the dialysis study and will disclose the result in due time. In the present study we have successfully tagged creatinine and urea to the INPs. In this communication, the detailed binding studies are disclosed.
BB and SKP conceived and designed the experiments. SKP performed the experiments. BB and SKP analyzed the data and drafted the manuscript. Both authors read and approved the final manuscript.
Biswadip Banerji received M.Sc. in Chemistry, University of Calcutta, Kolkata, India; Ph.D. degree from, Indian Institute of Technology, Kanpur, India; and he was a postdoctoral research fellow from Oxford Centre for Molecular Science and Chemistry Research Laboratory, Oxford University, UK; and postdoctoral research fellow from the Institute of Chemical & Engineering Sciences-Agency for Science, Technology and Research (ICES-A*STAR), Singapore. He was the Team Leader at TCG Lifesciences, Kolkata, India, prior to his current position as a Senior Scientist of Indian Institute of Chemical Biology (CSIR-IICB), Kolkata, India. His research area interests cover smart nano-biomaterials, peptide based drug designing, self-assembly of biomaterials and natural product inspired hybrid scaffolds and its application in therapeutics etc.
Sumit Kumar Pramanik obtained his B.Sc. in chemistry from Vidyasagar University, India. He earned his M.Sc. in applied chemistry from IIEST, Shibpur, India. He received his Ph.D. degree from Indian Institute of Chemical Biology, Kolkata, India under the mentorship of Dr. Biswadip Banerji. His research area interests include smart functionalized nanomaterials and peptide based drug design and biophysical chemistry.
SPK thanks CSIR-IICB, India for senior project fellowship. The authors would also like to thank CSIR-India, for generous funding in this work under network project NWP-0035 and the central instrumental facilities of CSIR-IICB.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Bachelet-Violette L, Silva AKA, Maire M, Michel A, Brinza O, Ou P, Ollivier V, Nicoletti A, Wilhelm C, Letourneur D, Menager C, Chaubet F (2014) Strong and specific interaction of ultra small superparamagnetic iron oxide nanoparticles and human activated platelets mediated by fucoidan coating. RSC Adv 4:4864–4871View ArticleGoogle Scholar
- Banerji B, Pramanik SK, Mandal S, Maiti NC, Chaudhuri K (2012a) Synthesis, characterization and cytotoxicity study of magnetic (Fe3O4) nanoparticles and their drug conjugate. RSC Ad 2:2493–2497View ArticleGoogle Scholar
- Banerji B, Pramanik SK, Pal U, Maiti NC (2012b) Conformation and cytotoxicity of a tetrapeptide constellated with alternative D- and L-proline. RSC Adv 2:6744–6747View ArticleGoogle Scholar
- Banerji B, Pramanik SK, Pal U, Maiti NC (2013) Dipeptide derived from benzylcystine forms unbranched nanotubes in aqueous solution. J Nanostructure Chemi 3:12View ArticleGoogle Scholar
- Banerji B, Pramanik SK, Pal U, Chandra Maiti N (2014) Binding of hemoglobin to ultrafine carbon nanoparticles: a spectroscopic insight into a major health hazard. RSC Adv 4:22536–22541View ArticleGoogle Scholar
- Brust M, Walker M, Bethell D, Schiffrin DJ, Whyman R (1994) Synthesis of thiol-derivatised gold nanoparticles in a two-phase liquid–liquid system. J Chem Soc Chem Commun 7:801–802View ArticleGoogle Scholar
- Chen S, Kimura K (1999) Synthesis and characterization of carboxylate-modified gold nanoparticle powders dispersible in water. Langmuir 15:1075–1082View ArticleGoogle Scholar
- Dalal P, Sangha H, Chaudhary K (2011) In peritoneal dialysis, is there sufficient evidence to make “PD First” therapy? Int J Nephrol 2011:239515View ArticleGoogle Scholar
- Dousdampanis P, Trigka K, Fourtounas C, Bargman JM (2014) Role of testosterone in the pathogenesis progression, prognosis and comorbidity of men with chronic kidney disease. Ther Apher Dial 18:220–230Google Scholar
- Fernández-Bertrán J, Alfonso L, Alvarez J, Reguera E (2000) Mechanochemical synthesis of urea adducts with long chain alkyl derivatives. J Inclusion Phenomena 37:131–136View ArticleGoogle Scholar
- Fischer PHH, McDowell CA (1960) The infrared absorption spectra of urea–hydrocarbon adducts. Can J Chem 38:187–193View ArticleGoogle Scholar
- Jerônimo D, de Souza R, da Silva F, Camargo G, Miranda H, Xavier M, Sakane K, Ribeiro W (2012) Detection of creatine in rat muscle by FTIR spectroscopy. Ann Biomed Eng 40:2069–2077View ArticleGoogle Scholar
- Jung YM, Czarnik-Matusewicz B, Kim SB (2004) Characterization of concentration-dependent infrared spectral variations of urea aqueous solutions by principal component analysis and two-dimensional correlation spectroscopy. J Phys Chem B 108:13008–13014View ArticleGoogle Scholar
- Kim S, Takayama S (2015) Organ-on-a-chip and the kidney. Kidney Res Clin Pract 34:165–169View ArticleGoogle Scholar
- Kuypers S, Pramanik SK, D’Olieslaeger L, Reekmans G, Peters M, D’Haen J, Vanderzande D, Junkers T, Adriaensens P, Ethirajan A (2015) Interfacial thiol-isocyanate reactions for functional nanocarriers: a facile route towards tunable morphologies and hydrophilic payload encapsulation. Chem Commun 51:15858–15861View ArticleGoogle Scholar
- Lin J, Li Y, Li Y, Wu H, Yu F, Zhou S, Xie L, Luo F, Lin C, Hou Z (2015) Drug/dye-loaded, multifunctional PEG–chitosan–iron oxide nanocomposites for methotraxate synergistically self-targeted cancer therapy and dual model imaging. ACS Appl Mater Interfaces 7:11908–11920View ArticleGoogle Scholar
- Na HB, Song IC, Hyeon T (2009) Inorganic nanoparticles for MRI contrast agents. Adv Mater 21:2133–2148View ArticleGoogle Scholar
- Nassar GM, Ayus JC (2001) Infectious complications of the hemodialysis access. Kidney Int 60:1–13View ArticleGoogle Scholar
- Nel AE, Madler L, Velegol D, Xia T, Hoek EMV, Somasundaran P, Klaessig F, Castranova V, Thompson M (2009) Understanding biophysicochemical interactions at the nano-bio interface. Nat Mater 8:543–557View ArticleGoogle Scholar
- Pezzaniti JL, Jeng T-W, McDowell L, Oosta GM (2001) Preliminary investigation of near-infrared spectroscopic measurements of urea, creatinine, glucose, protein, and ketone in urine. Clin Biochem 34:239–246View ArticleGoogle Scholar
- Rahbari-Oskoui F, Williams O, Chapman A (2014) Mechanisms and management of hypertension in autosomal dominant polycystic kidney disease. Nephrol Dial Transplant 12:2194–2201View ArticleGoogle Scholar
- Sakata Y, Shiraishi S, Otsuka M (2005) Effect of tablet geometrical structure on the dehydration of creatine monohydrate tablets, and their pharmaceutical properties. AAPS PharmSciTech 6:E527–E535View ArticleGoogle Scholar
- Sharifi S, Daghighi S, Motazacker MM, Badlou B, Sanjabi B, Akbarkhanzadeh A, Rowshani AT, Laurent S, Peppelenbosch MP, Rezaee F (2013) Superparamagnetic iron oxide nanoparticles alter expression of obesity and T2D-associated risk genes in human adipocytes. Sci Rep 3:2173View ArticleGoogle Scholar
- Todd T, Zhen Z, Tang W, Chen H, Wang G, Chuang Y-J, Deaton K, Pan Z, Xie J (2014) Iron oxide nanoparticle encapsulated diatoms for magnetic delivery of small molecules to tumors. Nanoscale 6:2073–2076View ArticleGoogle Scholar
- Trendafilova N, Kurbakova AP, Efimenko IA, Mitewa M, Bontchev PR (1991) Infrared spectra of Pt(II) creatinine complexes. Normal coordinate analysis of creatinine and Pt(creat)2(NO2)2. Spectrochim Acta Part A 47:577–584View ArticleGoogle Scholar
- Tromsdorf UI, Bruns OT, Salmen SC, Beisiegel U, Weller H (2009) A highly effective, nontoxic T1 MR contrast agent based on ultrasmall PEGylated iron oxide nanoparticles. Nano Lett 9:4434–4440View ArticleGoogle Scholar
- Verma ML, Puri M, Barrow CJ (2014) Recent trends in nanomaterials immobilised enzymes for biofuel production. Crit Rev Biotechnol pp 1–12Google Scholar
- Wahajuddin SA (2012) Superparamagnetic iron oxide nanoparticles: magnetic nanoplatforms as drug carriers. Int J Nanomed 7:3445–3471View ArticleGoogle Scholar
- Weingart J, Vabbilisetty P, Sun X-L (2013) Membrane mimetic surface functionalization of nanoparticles: methods and applications. Adv Colloid Interface Sci 197–198:68–84View ArticleGoogle Scholar
- Xie J, Wang J, Niu G, Huang J, Chen K, Li X, Chen X (2010) Human serum albumin coated iron oxide nanoparticles for efficient cell labeling. Chem Commun 46:433–435View ArticleGoogle Scholar